#------------------------------------------------------------------------------
#$Date: 2024-08-07 01:09:14 +0300 (Wed, 07 Aug 2024) $
#$Revision: 294012 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/57/06/1570609.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1570609
loop_
_publ_author_name
'Hogan-Lamarre, Pascal'
'Luo, Yi'
'Bücker, Robert'
'Miller, R. J. Dwayne'
'Zou, Xiaodong'
_publ_section_title
;
 STEM SerialED: achieving high-resolution data for ab initio structure
 determination of beam-sensitive nanocrystalline materials.
;
_journal_issue                   'Pt 1'
_journal_name_full               IUCrJ
_journal_page_first              62
_journal_page_last               72
_journal_paper_doi               10.1107/S2052252523009661
_journal_volume                  11
_journal_year                    2024
_chemical_formula_sum            'Na156 O2880 Si1440'
_chemical_formula_weight         90107.39
_chemical_name_systematic        ZSM-25
_space_group_crystal_system      cubic
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   43.269(5)
_cell_length_b                   43.269(5)
_cell_length_c                   43.269(5)
_cell_measurement_reflns_used    5740
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      0.637
_cell_measurement_theta_min      0.018
_cell_volume                     81008(16)
_computing_cell_refinement       'Diffractem and CrystFEL (Buecker et al. 2021)'
_computing_data_collection       'Instamatic (Smeets et al. 2018)'
_computing_data_reduction        'Diffractem and CrystFEL (Buecker et al. 2021)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Themis Z S/TEM 300kV'
_diffrn_measurement_method       SerialED
_diffrn_radiation_probe          electron
_diffrn_radiation_type           electron
_diffrn_radiation_wavelength     0.0196
_diffrn_reflns_av_R_equivalents  0.0
_diffrn_reflns_av_unetI/netI     0.1620
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_number            5740
_diffrn_reflns_point_group_measured_fraction_full 0.522
_diffrn_reflns_point_group_measured_fraction_max 0.522
_diffrn_reflns_theta_full        0.637
_diffrn_reflns_theta_max         0.637
_diffrn_reflns_theta_min         0.018
_diffrn_source                   electron
_exptl_absorpt_coefficient_mu    0.000
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            white
_exptl_crystal_density_diffrn    1.847
_exptl_crystal_description       cubic
_exptl_crystal_F_000             14832
_exptl_crystal_size_max          0.0005
_exptl_crystal_size_mid          0.0005
_exptl_crystal_size_min          0.0005
_refine_diff_density_max         0.489
_refine_diff_density_min         -0.347
_refine_diff_density_rms         0.077
_refine_ls_abs_structure_details
;
 All f" are zero, so absolute structure could not be determined
;
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.566
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     862
_refine_ls_number_reflns         5740
_refine_ls_number_restraints     1803
_refine_ls_restrained_S_all      1.403
_refine_ls_R_factor_all          0.3351
_refine_ls_R_factor_gt           0.2684
_refine_ls_shift/su_max          1.598
_refine_ls_shift/su_mean         0.041
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.2000P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.5468
_refine_ls_wR_factor_ref         0.5815
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    0.000
_reflns_Friedel_fraction_max     0.000
_reflns_number_gt                2888
_reflns_number_total             5740
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            of5002.cif
_cod_data_source_block           ZSM-25_I-43m_SerialED_calibratedUnitCell
_cod_depositor_comments
;Adding full bibliography for 1570607--1570609.cif.

 Adding full bibliography for 1570607--1570609.cif.
;
_cod_original_cell_volume        81010(29)
_cod_database_code               1570609
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y, x, z'
'-y, -x, z'
'y, -x, -z'
'-y, x, -z'
'x, z, y'
'-x, z, -y'
'-x, -z, y'
'x, -z, -y'
'z, y, x'
'z, -y, -x'
'-z, y, -x'
'-z, -y, x'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'z+1/2, x+1/2, y+1/2'
'z+1/2, -x+1/2, -y+1/2'
'-z+1/2, -x+1/2, y+1/2'
'-z+1/2, x+1/2, -y+1/2'
'y+1/2, z+1/2, x+1/2'
'-y+1/2, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x+1/2'
'-y+1/2, -z+1/2, x+1/2'
'y+1/2, x+1/2, z+1/2'
'-y+1/2, -x+1/2, z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-y+1/2, x+1/2, -z+1/2'
'x+1/2, z+1/2, y+1/2'
'-x+1/2, z+1/2, -y+1/2'
'-x+1/2, -z+1/2, y+1/2'
'x+1/2, -z+1/2, -y+1/2'
'z+1/2, y+1/2, x+1/2'
'z+1/2, -y+1/2, -x+1/2'
'-z+1/2, y+1/2, -x+1/2'
'-z+1/2, -y+1/2, x+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
O001 O 0.3484(8) 0.0407(5) 0.0407(5) 0.049(8) Uani 1 2 d DS TU P . .
O002 O 0.2085(6) 0.2085(6) 0.1519(8) 0.065(9) Uani 1 2 d DS TU P . .
O003 O 0.3472(5) 0.2631(4) 0.0427(5) 0.049(6) Uani 1 1 d D U . . .
O004 O 0.2115(5) 0.0732(4) 0.0105(3) 0.029(5) Uani 1 1 d D U . . .
O005 O 0.2392(5) 0.2392(5) 0.0669(8) 0.052(8) Uani 1 2 d DS TU P . .
O006 O 0.2358(6) 0.1828(4) 0.0418(5) 0.058(6) Uani 1 1 d D U . . .
O007 O 0.3212(8) 0.1811(6) 0.1811(6) 0.058(8) Uani 1 2 d DS TU P . .
O008 O 0.4322(6) 0.2607(4) 0.1832(5) 0.064(6) Uani 1 1 d D U . . .
O009 O 0.4621(8) 0.3765(5) 0.3765(5) 0.048(8) Uani 1 2 d DS TU P . .
O010 O 0.3817(3) 0.2416(6) 0.1515(6) 0.059(6) Uani 1 1 d D U . . .
O011 O 0.4303(5) 0.2060(4) 0.1532(5) 0.058(6) Uani 1 1 d D U . . .
O012 O 0.4304(5) 0.3500(4) 0.2680(6) 0.067(7) Uani 1 1 d D U . . .
O013 O 0.4306(8) 0.2927(6) 0.2927(6) 0.076(9) Uani 1 2 d DS TU P . .
O014 O 0.3197(6) 0.3197(6) 0.2634(7) 0.057(8) Uani 1 2 d DS TU P . .
O015 O 0.4917(3) 0.3540(5) 0.0422(6) 0.061(8) Uani 1 1 d D U . . .
Na15 Na 0.2906(15) 0.2906(15) 0.126(2) 0.18(4) Uiso 1 2 d S . P . .
O016 O 0.4564(5) 0.4564(5) 0.2923(8) 0.066(9) Uani 1 2 d DS TU P . .
O017 O 0.4276(5) 0.4276(5) 0.1469(8) 0.059(9) Uani 1 2 d DS TU P . .
O018 O 0.4603(4) 0.2402(4) 0.0699(5) 0.032(5) Uani 1 1 d D U . . .
O019 O 0.3461(5) 0.2545(6) 0.1025(3) 0.057(6) Uani 1 1 d D U . . .
O020 O 0.3814(4) 0.3128(6) 0.2618(6) 0.067(7) Uani 1 1 d D U . . .
Na20 Na 0.4954(15) 0.2677(13) 0.1739(14) 0.17(2) Uiso 1 1 d . . . . .
O021 O 0.4873(4) 0.4323(5) 0.3702(6) 0.058(7) Uani 1 1 d D U . . .
O022 O 0.4318(6) 0.2607(5) 0.1214(3) 0.059(6) Uani 1 1 d D U . . .
O023 O 0.4903(3) 0.1332(5) 0.0420(5) 0.034(6) Uani 1 1 d D U . . .
O024 O 0.4347(5) 0.0772(6) 0.0108(3) 0.062(8) Uani 1 1 d D U . . .
O025 O 0.3447(9) 0.2629(5) 0.2629(5) 0.063(9) Uani 1 2 d DS TU P . .
O026 O 0.1219(7) 0.0415(4) 0.0415(4) 0.026(7) Uani 1 2 d DS TU P . .
O027 O 0.4298(5) 0.3000(5) 0.0090(3) 0.048(7) Uani 1 1 d D U . . .
O028 O 0.4601(6) 0.4042(4) 0.2595(4) 0.054(6) Uani 1 1 d D U . . .
O029 O 0.4305(4) 0.3516(4) 0.0435(5) 0.049(6) Uani 1 1 d D U . . .
O030 O 0.4605(5) 0.4605(5) 0.0693(8) 0.049(8) Uani 1 2 d DS TU P . .
O031 O 0.2705(4) 0.2050(6) 0.1536(6) 0.061(6) Uani 1 1 d D U . . .
O032 O 0.3161(5) 0.3161(5) 0.0320(7) 0.033(6) Uani 1 2 d DS TU P . .
O033 O 0.4562(6) 0.3660(6) 0.2123(4) 0.069(7) Uani 1 1 d D U . . .
O034 O 0.2365(8) 0.1540(5) 0.1540(5) 0.062(9) Uani 1 2 d DS TU P . .
O035 O 0.3803(3) 0.0925(5) 0.0359(6) 0.047(6) Uani 1 1 d D U . . .
O036 O 0.4313(5) 0.2960(4) 0.0705(5) 0.052(6) Uani 1 1 d D U . . .
O037 O 0.3502(5) 0.3502(5) 0.1769(9) 0.076(9) Uani 1 2 d DS TU P . .
O038 O 0.4912(4) 0.3502(6) 0.2599(6) 0.071(8) Uani 1 1 d D U . . .
O039 O 0.3785(3) 0.3168(5) 0.0416(6) 0.052(6) Uani 1 1 d D U . . .
O040 O 0.0964(5) 0.0964(5) 0.0309(7) 0.034(8) Uani 1 2 d DS TU P . .
O041 O 0.2709(3) 0.1326(6) 0.0428(6) 0.053(6) Uani 1 1 d D U . . .
O042 O 0.2401(6) 0.1886(6) 0.1024(3) 0.061(7) Uani 1 1 d D U . . .
O043 O 0.4626(6) 0.4063(6) 0.1001(4) 0.061(7) Uani 1 1 d D U . . .
O044 O 0.3213(6) 0.1455(6) 0.0084(4) 0.062(8) Uani 1 1 d D U . . .
O045 O 0.3228(5) 0.1504(4) 0.0703(5) 0.049(6) Uani 1 1 d D U . . .
O046 O 0.4580(5) 0.4064(4) 0.0379(5) 0.050(6) Uani 1 1 d D U . . .
O047 O 0.4263(5) 0.4263(5) 0.3637(8) 0.049(8) Uani 1 2 d DS TU P . .
O048 O 0.3211(6) 0.1891(6) 0.1193(3) 0.052(6) Uani 1 1 d D U . . .
O049 O 0.4905(3) 0.2091(5) 0.1462(5) 0.052(7) Uani 1 1 d D U . . .
O050 O 0.3988(3) 0.2432(5) 0.0714(5) 0.045(6) Uani 1 1 d D U . . .
O051 O 0.4639(8) 0.1544(5) 0.1544(5) 0.056(8) Uani 1 2 d DS TU P . .
O052 O 0.4636(6) 0.4022(5) 0.3209(3) 0.058(7) Uani 1 1 d D U . . .
O053 O 0.4289(4) 0.1288(4) 0.0456(5) 0.042(6) Uani 1 1 d D U . . .
O054 O 0.4004(4) 0.3137(6) 0.1813(6) 0.069(7) Uani 1 1 d D U . . .
O055 O 0.4556(5) 0.1851(4) 0.0397(4) 0.033(5) Uani 1 1 d D U . . .
O056 O 0.4343(6) 0.2999(6) 0.2319(4) 0.066(7) Uani 1 1 d D U . . .
O057 O 0.4880(3) 0.4259(6) 0.1546(6) 0.068(8) Uani 1 1 d D U . . .
O058 O 0.4569(5) 0.1856(5) 0.0999(3) 0.041(6) Uani 1 1 d D U . . .
O059 O 0.3187(4) 0.0945(4) 0.0420(5) 0.048(6) Uani 1 1 d D U . . .
O060 O 0.2889(3) 0.2024(5) 0.0675(6) 0.056(6) Uani 1 1 d D U . . .
O061 O 0.2066(6) 0.0727(4) 0.0727(4) 0.020(5) Uani 1 2 d DS TU P . .
O062 O 0.3499(6) 0.2938(4) 0.1510(5) 0.072(7) Uani 1 1 d D U . . .
O063 O 0.3506(4) 0.2048(4) 0.0659(5) 0.047(6) Uani 1 1 d D U . . .
O064 O 0.3477(6) 0.2985(6) 0.2121(4) 0.076(7) Uani 1 1 d D U . . .
O065 O 0.4272(7) 0.0721(5) 0.0721(5) 0.046(8) Uani 1 2 d DS TU P . .
O066 O 0.3214(5) 0.2383(4) 0.1572(5) 0.061(6) Uani 1 1 d D U . . .
O067 O 0.2100(4) 0.1264(4) 0.0410(5) 0.032(5) Uani 1 1 d D U . . .
O068 O 0.4558(5) 0.3726(4) 0.1516(5) 0.061(7) Uani 1 1 d D U . . .
O069 O 0.4619(5) 0.3149(4) 0.1779(6) 0.073(7) Uani 1 1 d D U . . .
O070 O 0.1586(3) 0.0916(5) 0.0372(5) 0.026(5) Uani 1 1 d D U . . .
Si01 Si 0.3084(4) 0.2025(4) 0.1524(4) 0.042(5) Uani 1 1 d D U . . .
Si02 Si 0.3493(3) 0.2568(3) 0.1392(3) 0.025(4) Uani 1 1 d D U . . .
Si03 Si 0.4598(4) 0.1894(3) 0.1366(3) 0.042(5) Uani 1 1 d D U . . .
Si04 Si 0.4319(3) 0.2973(4) 0.1946(3) 0.039(5) Uani 1 1 d D U . . .
Si05 Si 0.4714(4) 0.2040(3) 0.0693(3) 0.043(5) Uani 1 1 d D U . . .
Si06 Si 0.4306(4) 0.2603(4) 0.0832(4) 0.051(5) Uani 1 1 d D U . . .
Si07 Si 0.4192(4) 0.3142(4) 0.2639(4) 0.062(6) Uani 1 1 d D U . . .
Si08 Si 0.1267(3) 0.0748(3) 0.0245(3) 0.040(5) Uani 1 1 d D U . . .
Si09 Si 0.3627(3) 0.3156(3) 0.1819(3) 0.041(5) Uani 1 1 d D U . . .
Si10 Si 0.3084(3) 0.1309(3) 0.0408(3) 0.031(4) Uani 1 1 d D U . . .
Si11 Si 0.4605(4) 0.3696(4) 0.0278(4) 0.056(6) Uani 1 1 d D U . . .
Si12 Si 0.4590(4) 0.3675(4) 0.2501(4) 0.044(5) Uani 1 1 d D U . . .
Si13 Si 0.3474(3) 0.0772(3) 0.0245(3) 0.028(4) Uani 1 1 d D U . . .
Si14 Si 0.3488(3) 0.2978(3) 0.0266(3) 0.021(4) Uani 1 1 d D U . . .
Si15 Si 0.3484(4) 0.2989(3) 0.2500(4) 0.051(6) Uani 1 1 d D U . . .
Si16 Si 0.4588(4) 0.4083(3) 0.1376(4) 0.046(5) Uani 1 1 d D U . . .
Si17 Si 0.3610(3) 0.2411(3) 0.0703(3) 0.032(4) Uani 1 1 d D U . . .
Si18 Si 0.4190(3) 0.2426(3) 0.1524(3) 0.028(4) Uani 1 1 d D U . . .
Si19 Si 0.4600(4) 0.4092(3) 0.3581(4) 0.047(6) Uani 1 1 d D U . . .
Si20 Si 0.4728(4) 0.4244(3) 0.0679(3) 0.038(5) Uani 1 1 d D U . . .
Si21 Si 0.2385(3) 0.1894(3) 0.1402(3) 0.036(5) Uani 1 1 d D U . . .
Si22 Si 0.2511(4) 0.2036(4) 0.0690(4) 0.043(5) Uani 1 1 d D U . . .
Si23 Si 0.4174(3) 0.0924(3) 0.0417(3) 0.034(5) Uani 1 1 d D U . . .
Si24 Si 0.2391(4) 0.1470(4) 0.0286(4) 0.059(6) Uani 1 1 d D U . . .
Si25 Si 0.4708(4) 0.3519(4) 0.1800(4) 0.052(5) Uani 1 1 d D U . . .
Si26 Si 0.4166(4) 0.3162(4) 0.0418(4) 0.050(5) Uani 1 1 d D U . . .
Si27 Si 0.4572(3) 0.1484(3) 0.0290(3) 0.026(4) Uani 1 1 d D U . . .
Si28 Si 0.3206(4) 0.1869(4) 0.0817(4) 0.045(5) Uani 1 1 d D U . . .
Si29 Si 0.1969(3) 0.0911(3) 0.0411(3) 0.031(4) Uani 1 1 d D U . . .
Si30 Si 0.4730(4) 0.4224(3) 0.2898(4) 0.050(6) Uani 1 1 d D U . . .
Na1 Na 0.5089(9) 0.4911(9) 0.2793(13) 0.020(15) Uiso 0.5 2 d S . P . .
Na2 Na 0.3440(7) 0.1122(5) 0.1122(5) 0.020(7) Uiso 1 2 d S . P . .
Na5 Na 0.4369(7) 0.2276(5) 0.2276(5) 0.020(7) Uiso 1 2 d S . P . .
Na4 Na 0.3716(7) 0.3716(7) 0.0487(10) 0.057(12) Uiso 1 2 d S . P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Si13 O001 Si13 137.8(18) 17 . ?
Si21 O002 Si21 136(2) 13 . ?
Si17 O003 Si14 144.8(16) . . ?
Si17 O003 Na20 113.8(17) . 48_554 ?
Si14 O003 Na20 98.4(16) . 48_554 ?
Si30 O004 Si29 136.4(14) 48_554 . ?
Si22 O005 Si22 126(2) . 13 ?
Si22 O006 Si24 137.1(16) . . ?
Si01 O007 Si01 138(2) 17 . ?
Si18 O008 Si04 133.8(15) . . ?
Si18 O008 Na5 113.0(12) . . ?
Si04 O008 Na5 109.5(12) . . ?
Si19 O009 Si19 148(2) . 17 ?
Si18 O010 Si02 148.6(17) . . ?
Si03 O011 Si18 130.2(14) . . ?
Si07 O012 Si12 127.5(15) . . ?
Si07 O013 Si07 141(2) 17 . ?
Si15 O014 Si15 135(2) . 13 ?
Si27 O015 Si11 149.0(18) 46 . ?
Si02 Na15 Si02 143(3) . 13 ?
Si30 O016 Si30 141(2) 13 . ?
Si16 O017 Si16 141(2) . 13 ?
Si05 O018 Si06 137.4(14) . . ?
Si02 O019 Si17 146.5(16) . . ?
Si15 O020 Si07 154.9(19) . . ?
O069 Na20 O003 153(3) . 46 ?
Si19 O021 Si08 128.3(15) . 46 ?
Si18 O022 Si06 143.0(16) . . ?
Si11 O023 Si27 149.3(16) 46 . ?
Si20 O024 Si23 141.7(16) 48_554 . ?
Si15 O025 Si15 128(2) 17 . ?
Si08 O026 Si08 141(2) . 17 ?
Si05 O027 Si26 153.0(16) 48_554 . ?
Si30 O028 Si12 132.7(15) . . ?
Si26 O029 Si11 134.7(15) . . ?
Si20 O030 Si20 127(2) 13 . ?
Si21 O031 Si01 143.2(17) . . ?
Si14 O032 Si14 145(2) 13 . ?
Si12 O033 Si25 146.1(17) . . ?
Si21 O034 Si21 132(2) . 17 ?
Si23 O035 Si13 154.3(17) . . ?
Si06 O036 Si26 138.2(15) . . ?
Si09 O037 Si09 127(2) . 13 ?
Si24 O038 Si12 145.0(17) 46 . ?
Si26 O039 Si14 140.2(15) . . ?
Si26 O039 Na4 98.0(12) . . ?
Si14 O039 Na4 116.4(14) . . ?
Si08 O040 Si08 153(2) 13 . ?
Si10 O041 Si24 146.9(17) . . ?
Si21 O042 Si22 151.4(18) . . ?
Si16 O043 Si20 146.8(17) . . ?
Si25 O044 Si10 150.3(17) 48_554 . ?
Si10 O045 Si28 133.8(15) . . ?
Si10 O045 Na2 110.3(11) . . ?
Si28 O045 Na2 114.6(12) . . ?
Si20 O046 Si11 129.7(14) . . ?
Si19 O047 Si19 140(2) . 13 ?
Si28 O048 Si01 152.6(17) . . ?
Si14 O049 Si03 136.9(15) 46 . ?
Si17 O050 Si06 150.3(16) . . ?
Si03 O051 Si03 142(2) . 17 ?
Si19 O052 Si30 136.0(16) . . ?
Si27 O053 Si23 131.9(14) . . ?
Si09 O054 Si04 147.6(18) . . ?
Si27 O055 Si05 132.0(13) . . ?
Si04 O056 Si07 146.6(17) . . ?
Si13 O057 Si16 134.3(16) 46 . ?
Si03 O058 Si05 135.3(14) . . ?
Si13 O059 Si10 129.2(14) . . ?
Si22 O060 Si28 146.3(17) . . ?
Si29 O061 Si29 138.7(19) 17 . ?
Si02 O062 Si09 139.4(15) . . ?
Si17 O063 Si28 127.7(14) . . ?
Si09 O064 Si15 141.9(18) . . ?
Si23 O065 Si23 143(2) 17 . ?
Si02 O066 Si01 130.1(15) . . ?
Si29 O067 Si24 141.3(15) . . ?
Si25 O068 Si16 138.0(16) . . ?
Si25 O069 Si04 126.9(15) . . ?
Si25 O069 Na20 131.1(19) . . ?
Si04 O069 Na20 96.2(17) . . ?
Si08 O070 Si29 149.2(14) . . ?
O048 Si01 O007 110.4(15) . . ?
O048 Si01 O031 112.5(14) . . ?
O007 Si01 O031 110.4(15) . . ?
O048 Si01 O066 109.1(13) . . ?
O007 Si01 O066 108.5(14) . . ?
O031 Si01 O066 105.8(12) . . ?
O019 Si02 O010 111.7(13) . . ?
O019 Si02 O066 112.1(13) . . ?
O010 Si02 O066 106.2(13) . . ?
O019 Si02 O062 111.3(13) . . ?
O010 Si02 O062 105.7(12) . . ?
O066 Si02 O062 109.5(12) . . ?
O019 Si02 Na15 76(2) . . ?
O010 Si02 Na15 171(2) . . ?
O066 Si02 Na15 73(2) . . ?
O062 Si02 Na15 66.8(19) . . ?
O058 Si03 O011 115.0(13) . . ?
O058 Si03 O049 111.5(12) . . ?
O011 Si03 O049 107.0(12) . . ?
O058 Si03 O051 111.6(13) . . ?
O011 Si03 O051 105.9(13) . . ?
O049 Si03 O051 105.2(14) . . ?
O056 Si04 O054 111.9(14) . . ?
O056 Si04 O008 111.2(13) . . ?
O054 Si04 O008 108.4(13) . . ?
O056 Si04 O069 110.5(14) . . ?
O054 Si04 O069 107.2(13) . . ?
O008 Si04 O069 107.5(13) . . ?
O018 Si05 O027 113.0(13) . 46 ?
O018 Si05 O055 111.3(12) . . ?
O027 Si05 O055 111.9(13) 46 . ?
O018 Si05 O058 109.6(12) . . ?
O027 Si05 O058 107.5(13) 46 . ?
O055 Si05 O058 102.8(12) . . ?
O036 Si06 O050 109.6(13) . . ?
O036 Si06 O022 108.9(13) . . ?
O050 Si06 O022 109.8(13) . . ?
O036 Si06 O018 111.6(13) . . ?
O050 Si06 O018 107.6(12) . . ?
O022 Si06 O018 109.2(13) . . ?
O013 Si07 O012 111.5(15) . . ?
O013 Si07 O020 108.9(16) . . ?
O012 Si07 O020 109.9(14) . . ?
O013 Si07 O056 107.8(16) . . ?
O012 Si07 O056 109.2(14) . . ?
O020 Si07 O056 109.6(14) . . ?
O026 Si08 O040 109.0(14) . . ?
O026 Si08 O021 106.7(12) . 48_554 ?
O040 Si08 O021 109.8(15) . 48_554 ?
O026 Si08 O070 110.0(13) . . ?
O040 Si08 O070 111.2(14) . . ?
O021 Si08 O070 110.0(13) 48_554 . ?
O037 Si09 O054 112.3(13) . . ?
O037 Si09 O064 113.2(15) . . ?
O054 Si09 O064 112.8(14) . . ?
O037 Si09 O062 107.3(16) . . ?
O054 Si09 O062 106.4(13) . . ?
O064 Si09 O062 104.1(12) . . ?
O041 Si10 O044 111.9(13) . . ?
O041 Si10 O059 108.2(12) . . ?
O044 Si10 O059 107.8(13) . . ?
O041 Si10 O045 108.2(13) . . ?
O044 Si10 O045 109.6(13) . . ?
O059 Si10 O045 111.2(12) . . ?
O015 Si11 O023 113.8(13) . 48_554 ?
O015 Si11 O046 110.6(13) . . ?
O023 Si11 O046 109.3(12) 48_554 . ?
O015 Si11 O029 107.3(13) . . ?
O023 Si11 O029 108.7(13) 48_554 . ?
O046 Si11 O029 107.0(13) . . ?
O028 Si12 O038 110.8(14) . . ?
O028 Si12 O033 106.9(13) . . ?
O038 Si12 O033 107.5(14) . . ?
O028 Si12 O012 110.4(13) . . ?
O038 Si12 O012 107.8(13) . . ?
O033 Si12 O012 113.4(14) . . ?
O057 Si13 O059 117.2(13) 48_554 . ?
O057 Si13 O035 112.3(13) 48_554 . ?
O059 Si13 O035 109.6(13) . . ?
O057 Si13 O001 109.2(13) 48_554 . ?
O059 Si13 O001 104.5(12) . . ?
O035 Si13 O001 102.9(13) . . ?
O049 Si14 O032 110.2(14) 48_554 . ?
O049 Si14 O003 104.3(12) 48_554 . ?
O032 Si14 O003 110.2(13) . . ?
O049 Si14 O039 111.5(13) 48_554 . ?
O032 Si14 O039 111.8(14) . . ?
O003 Si14 O039 108.6(12) . . ?
O020 Si15 O014 110.5(15) . . ?
O020 Si15 O064 109.3(14) . . ?
O014 Si15 O064 110.2(15) . . ?
O020 Si15 O025 109.0(16) . . ?
O014 Si15 O025 109.0(16) . . ?
O064 Si15 O025 108.8(14) . . ?
O043 Si16 O017 110.8(15) . . ?
O043 Si16 O057 113.2(14) . . ?
O017 Si16 O057 106.6(15) . . ?
O043 Si16 O068 108.7(13) . . ?
O017 Si16 O068 108.5(14) . . ?
O057 Si16 O068 109.0(13) . . ?
O003 Si17 O019 105.8(13) . . ?
O003 Si17 O050 110.7(13) . . ?
O019 Si17 O050 110.4(13) . . ?
O003 Si17 O063 111.6(13) . . ?
O019 Si17 O063 109.2(13) . . ?
O050 Si17 O063 109.1(12) . . ?
O010 Si18 O008 112.2(14) . . ?
O010 Si18 O022 109.1(13) . . ?
O008 Si18 O022 108.4(12) . . ?
O010 Si18 O011 105.8(12) . . ?
O008 Si18 O011 109.6(13) . . ?
O022 Si18 O011 111.8(13) . . ?
O009 Si19 O021 109.6(15) . . ?
O009 Si19 O052 108.1(13) . . ?
O021 Si19 O052 111.2(14) . . ?
O009 Si19 O047 111.3(16) . . ?
O021 Si19 O047 108.7(14) . . ?
O052 Si19 O047 107.9(15) . . ?
O046 Si20 O024 108.4(13) . 46 ?
O046 Si20 O030 110.6(14) . . ?
O024 Si20 O030 111.1(13) 46 . ?
O046 Si20 O043 109.7(13) . . ?
O024 Si20 O043 107.6(13) 46 . ?
O030 Si20 O043 109.3(14) . . ?
O002 Si21 O042 110.8(15) . . ?
O002 Si21 O034 108.6(16) . . ?
O042 Si21 O034 110.2(13) . . ?
O002 Si21 O031 110.8(15) . . ?
O042 Si21 O031 108.8(14) . . ?
O034 Si21 O031 107.6(15) . . ?
O006 Si22 O005 110.9(15) . . ?
O006 Si22 O060 111.1(14) . . ?
O005 Si22 O060 110.1(13) . . ?
O006 Si22 O042 107.5(13) . . ?
O005 Si22 O042 109.2(15) . . ?
O060 Si22 O042 107.9(13) . . ?
O035 Si23 O065 112.4(15) . . ?
O035 Si23 O053 108.2(12) . . ?
O065 Si23 O053 110.5(13) . . ?
O035 Si23 O024 108.7(13) . . ?
O065 Si23 O024 108.3(14) . . ?
O053 Si23 O024 108.6(12) . . ?
O038 Si24 O067 113.1(14) 48_554 . ?
O038 Si24 O041 112.5(14) 48_554 . ?
O067 Si24 O041 108.5(13) . . ?
O038 Si24 O006 105.8(13) 48_554 . ?
O067 Si24 O006 109.3(13) . . ?
O041 Si24 O006 107.4(13) . . ?
O044 Si25 O033 112.7(14) 46 . ?
O044 Si25 O069 107.4(13) 46 . ?
O033 Si25 O069 108.5(14) . . ?
O044 Si25 O068 109.1(14) 46 . ?
O033 Si25 O068 106.1(13) . . ?
O069 Si25 O068 113.1(14) . . ?
O036 Si26 O029 108.5(13) . . ?
O036 Si26 O039 113.5(14) . . ?
O029 Si26 O039 110.4(12) . . ?
O036 Si26 O027 106.6(13) . . ?
O029 Si26 O027 107.5(13) . . ?
O039 Si26 O027 110.0(13) . . ?
O015 Si27 O053 114.3(13) 48_554 . ?
O015 Si27 O055 109.9(12) 48_554 . ?
O053 Si27 O055 109.9(12) . . ?
O015 Si27 O023 107.2(12) 48_554 . ?
O053 Si27 O023 106.7(12) . . ?
O055 Si27 O023 108.6(12) . . ?
O048 Si28 O060 111.1(14) . . ?
O048 Si28 O063 112.0(14) . . ?
O060 Si28 O063 108.0(13) . . ?
O048 Si28 O045 110.5(13) . . ?
O060 Si28 O045 109.0(13) . . ?
O063 Si28 O045 106.1(12) . . ?
O067 Si29 O061 111.8(13) . . ?
O067 Si29 O004 107.7(12) . . ?
O061 Si29 O004 109.9(13) . . ?
O067 Si29 O070 109.6(12) . . ?
O061 Si29 O070 110.0(13) . . ?
O004 Si29 O070 107.7(12) . . ?
O028 Si30 O004 111.6(14) . 46 ?
O028 Si30 O016 109.6(15) . . ?
O004 Si30 O016 109.4(13) 46 . ?
O028 Si30 O052 108.3(13) . . ?
O004 Si30 O052 109.6(14) 46 . ?
O016 Si30 O052 108.2(15) . . ?
O045 Na2 O045 138.8(16) . 17 ?
O008 Na5 O008 160.9(16) . 17 ?
O039 Na4 O039 103.0(17) 13 . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
O001 Si13 1.727(12) 17 ?
O001 Si13 1.727(12) . ?
O002 Si21 1.621(15) 13 ?
O002 Si21 1.621(15) . ?
O003 Si17 1.639(15) . ?
O003 Si14 1.656(15) . ?
O003 Na20 2.61(6) 48_554 ?
O004 Si30 1.635(16) 48_554 ?
O004 Si29 1.658(15) . ?
O005 Si22 1.626(15) . ?
O005 Si22 1.626(15) 13 ?
O006 Si22 1.624(16) . ?
O006 Si24 1.658(16) . ?
O007 Si01 1.644(15) 17 ?
O007 Si01 1.644(15) . ?
O008 Si18 1.648(16) . ?
O008 Si04 1.657(16) . ?
O008 Na5 2.40(2) . ?
O009 Si19 1.627(15) . ?
O009 Si19 1.627(15) 17 ?
O010 Si18 1.616(16) . ?
O010 Si02 1.637(15) . ?
O011 Si03 1.631(16) . ?
O011 Si18 1.656(16) . ?
O012 Si07 1.635(17) . ?
O012 Si12 1.645(16) . ?
O013 Si07 1.633(16) 17 ?
O013 Si07 1.633(16) . ?
O014 Si15 1.639(15) . ?
O014 Si15 1.639(15) 13 ?
O015 Si27 1.618(15) 46 ?
O015 Si11 1.632(16) . ?
Na15 Si02 2.99(3) . ?
Na15 Si02 2.99(3) 13 ?
O016 Si30 1.643(15) 13 ?
O016 Si30 1.643(15) . ?
O017 Si16 1.639(16) . ?
O017 Si16 1.639(16) 13 ?
O018 Si05 1.634(16) . ?
O018 Si06 1.658(16) . ?
O019 Si02 1.598(15) . ?
O019 Si17 1.639(16) . ?
O020 Si15 1.631(16) . ?
O020 Si07 1.639(17) . ?
Na20 O069 2.51(6) . ?
Na20 O003 2.61(6) 46 ?
O021 Si19 1.631(16) . ?
O021 Si08 1.641(16) 46 ?
O022 Si18 1.651(16) . ?
O022 Si06 1.653(16) . ?
O023 Si11 1.633(16) 46 ?
O023 Si27 1.672(15) . ?
O024 Si20 1.650(16) 48_554 ?
O024 Si23 1.670(16) . ?
O025 Si15 1.662(16) 17 ?
O025 Si15 1.662(16) . ?
O026 Si08 1.633(15) . ?
O026 Si08 1.633(15) 17 ?
O027 Si05 1.637(16) 48_554 ?
O027 Si26 1.685(16) . ?
O028 Si30 1.628(16) . ?
O028 Si12 1.639(16) . ?
O029 Si26 1.648(16) . ?
O029 Si11 1.660(16) . ?
O030 Si20 1.654(15) 13 ?
O030 Si20 1.654(15) . ?
O031 Si21 1.645(16) . ?
O031 Si01 1.647(16) . ?
O032 Si14 1.637(14) 13 ?
O032 Si14 1.637(14) . ?
O033 Si12 1.641(16) . ?
O033 Si25 1.649(16) . ?
O034 Si21 1.646(15) . ?
O034 Si21 1.646(15) 17 ?
O035 Si23 1.623(15) . ?
O035 Si13 1.646(15) . ?
O036 Si06 1.639(16) . ?
O036 Si26 1.644(16) . ?
O037 Si09 1.609(15) . ?
O037 Si09 1.609(15) 13 ?
O038 Si24 1.622(17) 46 ?
O038 Si12 1.641(16) . ?
O039 Si26 1.650(16) . ?
O039 Si14 1.659(15) . ?
O039 Na4 2.41(3) . ?
O040 Si08 1.634(14) 13 ?
O040 Si08 1.634(14) . ?
O041 Si10 1.624(16) . ?
O041 Si24 1.632(16) . ?
O042 Si21 1.638(16) . ?
O042 Si22 1.653(16) . ?
O043 Si16 1.630(16) . ?
O043 Si20 1.660(16) . ?
O044 Si25 1.632(16) 48_554 ?
O044 Si10 1.634(16) . ?
O045 Si10 1.652(16) . ?
O045 Si28 1.661(16) . ?
O045 Na2 2.62(2) . ?
O046 Si20 1.642(16) . ?
O046 Si11 1.654(16) . ?
O047 Si19 1.655(15) . ?
O047 Si19 1.655(15) 13 ?
O048 Si28 1.631(16) . ?
O048 Si01 1.640(16) . ?
O049 Si14 1.605(16) 46 ?
O049 Si03 1.635(16) . ?
O050 Si17 1.639(16) . ?
O050 Si06 1.645(16) . ?
O051 Si03 1.707(12) . ?
O051 Si03 1.707(12) 17 ?
O052 Si19 1.643(16) . ?
O052 Si30 1.658(16) . ?
O053 Si27 1.651(15) . ?
O053 Si23 1.659(16) . ?
O054 Si09 1.631(16) . ?
O054 Si04 1.643(16) . ?
O055 Si27 1.654(15) . ?
O055 Si05 1.667(16) . ?
O056 Si04 1.621(16) . ?
O056 Si07 1.652(16) . ?
O057 Si13 1.590(15) 46 ?
O057 Si16 1.647(16) . ?
O058 Si03 1.598(15) . ?
O058 Si05 1.668(16) . ?
O059 Si13 1.634(16) . ?
O059 Si10 1.640(16) . ?
O060 Si22 1.639(16) . ?
O060 Si28 1.646(16) . ?
O061 Si29 1.635(14) 17 ?
O061 Si29 1.635(14) . ?
O062 Si02 1.681(15) . ?
O062 Si09 1.725(15) . ?
O063 Si17 1.643(16) . ?
O063 Si28 1.660(16) . ?
O064 Si09 1.637(16) . ?
O064 Si15 1.643(16) . ?
O065 Si23 1.638(14) 17 ?
O065 Si23 1.638(14) . ?
O066 Si02 1.645(16) . ?
O066 Si01 1.659(16) . ?
O067 Si29 1.628(16) . ?
O067 Si24 1.632(16) . ?
O068 Si25 1.656(16) . ?
O068 Si16 1.666(16) . ?
O069 Si25 1.650(16) . ?
O069 Si04 1.668(16) . ?
O070 Si08 1.652(15) . ?
O070 Si29 1.667(15) . ?
Si05 O027 1.637(16) 46 ?
Si08 O021 1.641(16) 48_554 ?
Si11 O023 1.633(16) 48_554 ?
Si13 O057 1.590(15) 48_554 ?
Si14 O049 1.605(16) 48_554 ?
Si20 O024 1.650(16) 46 ?
Si24 O038 1.622(17) 48_554 ?
Si25 O044 1.632(16) 46 ?
Si27 O015 1.618(15) 48_554 ?
Si30 O004 1.635(16) 46 ?
Na1 Na1 1.09(11) 2_665 ?
Na2 O045 2.62(2) 17 ?
Na5 O008 2.40(2) 17 ?
Na4 O039 2.41(3) 13 ?
loop_
_cod_changelog_entry_id
_cod_changelog_entry_author
_cod_changelog_entry_date
_cod_changelog_entry_text
1 'Vaitkus, Antanas' 2024-05-07T16:33:00+03:00
;
 Marked entry as measured using electrons as the radiation probe.
 Updated bibliographic information.
;
